2D MXenes Embedded Perovskite Hydrogels for Efficient and Stable Solar Evaporation

Abstract Solar evaporation is a facile and promising technology to efficiently utilize renewable energy for freshwater production and seawater desalination. Here, the fabrication of self‐regenerating hydrogel composed of 2D‐MXenes nanosheets embedded in perovskite La 0.6Sr 0.4Co 0.2Fe 0.8O3− δ (LSCF)/polyvinyl alcohol hydrogels for efficient solar‐driven evaporation and seawater desalination is reported. The mixed dimensional LSCF/Ti3C2 composite features a localized surface plasmonic resonance effect in the polymeric network of polyvinyl alcohol endows excellent evaporation rates (1.98 kg m−2 h−1) under 1 k Wm−2 or one sun solar irradiation ascribed by hydrophilicity and broadband solar absorption (96%). Furthermore, the long‐term performance reveals smooth mass change (13.33 kg m−2) during 8 h under one sun. The composite hydrogel prompts the dilution of concentrated brines and redissolves it back to water (1.2 g NaCl/270 min) without impeding the evaporation rate without any salt‐accumulation. The present research offers a substantial opportunity for solar‐driven evaporation without any salt accumulation in real‐life applications.


Introduction
Water scarcity has increased severalfold in the past few decades with the advancement in the lifestyle and industrial sectors.[15][16][17][18][19] However, there still exists a substantial barrier between the status quo and industrial implications owing to the low solar absorption, poor thermal management, and structural deformation due to salt accumulation inside hydrophilic water channels of solar desalination devices when operated under seawater.
[22][23] Considerably, the heat energy provided by photothermal materials is a concentrated form of energy to boost the charge transportation for photogenerated carriers.[26][27] Several photothermal materials have been explored, i.e., carbon-based materials, [17,18,[28][29][30][31][32] plasmonic metallic nanoparticle, [33][34][35][36] semiconductors, [37][38][39] and polymers-based materials [40][41][42] has been reported in the development of efficient solar powered water desalination devices.Lanthanum strontium cobalt iron oxide (La 1−x Sr x Co 1−y Fe y O 3 ) is a specific ceramic oxide widely used as perovskite material and recognized for its high ionic and electronic conductivities and used as membrane materials for possessing good chemical/phase stability as well as high oxygen permeability. [43,44]t has been extensively explored as magnetic, [45] catalytic, [46] solid oxide fuel cells, [47] and dielectric properties.Zhao et al. reported the Lanthanum strontium cobalt iron oxide (LSCF) and 3DOM (3D ordered macro-porous structure) for synergistic photo/thermos-catalytic effect for CO 2 reduction and achieved a high temperature due to the photothermal effect leading toward high efficiency.The high photothermal effect of such materials can also be exploited for enhanced solar steam generation. [46]ecently, Ti 3 C 2 (MXenes), a newly discovered 2D transition metal material has been extensively studied in a variety of applications owing to its excellent electronic conduction with good charge transportation, optimized solar absorption, and numerous hydrophilic groups endorsing its hydrophilicity and strong coupling with other materials. [48,49]MXenes are generally represented by the M n+1 X n T z , where T z denotes the surface terminations of various groups, i.e., ─O, ─OH, and/or ─F.In fact, these surface terminations facilitate the spontaneous ion intercalation and exchange among 2D nanosheets and bestow it hydrophilicity.More interestingly, these 2D materials can be freely combined with other materials to form layered compounds, which opens the door to the development of novel functional materials and devices. [50,51]This approach offers great promise for tailoring the electronic states allowing for more flexibility and tailoring the unique 2D electronic states with atomic-scale accuracy, allowing for more flexibility in 2D materials and devices by stacking any number of atomically thin layers.
Herein, we report the fabrication of salt-resistance photothermal hydrogel for seawater desalination prepared by interpenetrating the La 0.6 Sr 0.4 Co 0.2 Fe 0.8 O 3− (LSCF) and Ti 3 C 2 (MXenes) into a polymeric network of polyvinyl alcohol (PVA) to enable the enhanced photothermal conversion with minimum thermal conduction.The 2D nanosheets of MXene facilitate the maximum light capture with the combination of perovskite oxide nanocomposite.Moreover, skeletons of polymeric networks with the porous channels of hydrogel additives endow the LSCF/Ti 3 C 2 with ample water content, good thermal management, and high salt resistance for effective solar vapor production, as schematically illustrated in Figure 1.
The prepared device manifested excellent thermal management with a minimum thermal conductivity value of 0.10 049 Wm −1 K −1 to confine heat over the top surface.The photothermal LSCF/Ti 3 C 2 hydrogel manifests a high evaporation rate of up to ≈1.98 kg m −2 h −1 under 1 k Wm −2 with ≈90.6% evaporation efficiency.State-of-the-art evaporation performances under different brine concentrations validate its self-regenerating/rejection efficiency.Based on these merits, the utilization of the perovskite incorporated 2D material composite benefits the enhanced photothermal conversion efficiency to evade surface fouling and achieve long-term stability (13.33 kg m −2 mass change yields during 8 h under one sun) for sustainable seawater desalination.

Results and Discussion
Harvesting solar energy by photon absorption via a novel combination of materials and collecting the photogenerated hot electrons as a result of internal photoemission has been explored extensively for efficient and stable solar-driven applications.The LSCF nanoparticles were in situ embedded on the 2D MXenes nanosheets via the facile hydrothermal method.The elemental composition and chemical states of the as-prepared LSCF/Ti 3 C 2 powder were affirmed using X-ray photoelectron spectroscopy (XPS).The whole XPS scan of LSCF/Ti 3 C 2 is shown in Figure 2a, revealing the presence of the Ti3p, Sr3d, Sr3p, C1s, Ti2p, O1s, Fe2p, Co2p, and La3d, respectively.
The high-resolution spectrum of Ti2p is shown in Figure 2b.The peak fitting of Ti2p confirms the existence of multiple bonds, i.e., TiO 2 (459.1 eV), Ti 2+ (461.21eV), TiC (464.61 eV), Ti 2+ (455.47 eV), and TiO 2 (455.06 eV) due to spin-orbit splitting of 2p into 2p 3/2 and 2p 1/2 , respectively. [19]Figure 2c shows the XPS spectrum of 3d states of La which is split and forms a double structure.Mainly, the spin-orbit coupling causes the La3d states to split into 3d 5/2 and 3d 3/2 states.Each state is further split into multiple components 3d 3/2 (833.09,835.14, 837.64 eV) and 3d 5/2 (850.19,853.96 eV) due to electron transfer to the La 4f from oxygen ligands. [19]The XPS spectrum of Sr3d shows multiple components, including 3d 3/2, and 3d 5/2, components (Figure 2d).The peaks at 131.72 and 132.86 eV correspond to the 3d 5/2 orbital and at 133.43 and 134.64 eV are attributed to the 3d 5/2 orbital. [19]he 2p peak fitting of Fe was performed according to the constraints for Fe 3+ and Fe 2+ .The Fe2p spectrum of LSCF shows four prominent peaks at 709.08, 711.03 eV (corresponding to 2p 3/2 orbital), 722.80, and 723.94 eV (corresponding to 2p 1/2 ), as shown in Figure 2e.The existence of the trance quantities of Fe 4+ could lead the second component of iron (Fe 3+ ) to possess relatively higher binding energy values. [52]Moreover, the surface functionality of the LSCF/Ti 3 C 2 was assessed by performing FTIR spectroscopy.The FTIR spectrum of LSCF/Ti 3 C 2 is given in Figure 2f.The peaks that appeared at 608.42 and 767.61 cm −1 are due to the presence of La─O, Sr─O, and H─Sr─OH bonds. [52]The peaks from 1000 to 1700 cm −1 may be attributed to the O─H bond vibrations and stretching of the C─F bond, respectively.Whereas, the absorption peaks at 2145.34 and 2822.20 cm −1 are attributed to the stretching vibrations of asymmetric and symmetric bonds of C─H. [53]A wide peak appearing at 3431.98 cm −1 is attributed to the stretching band of O─H, indicating the adsorption of water molecules. [53]he microstructural and surface morphologies of the prepared MXenes (Ti 3 C 2 ), LSCF, and LSCF/Ti 3 C 2 hydrogel were inspected using advanced field emission scanning electron microscopy (FE-SEM).Figure 3a shows the morphology of the 2D exfoliated MXenes (Ti 3 C 2 ) nanosheets which shows the etching using the strong etchant HF aqueous solution to selectively eliminate the aluminum layers, which results in nanoarches at the edges of the exfoliated Ti 3 C 2 planes.The Van Der Waals forces among 2D planar layers of Ti 3 C 2 impart a zipping morphological structure that follows a regular and smooth morphology facilitating enhanced surface-to-volume ratio and active sites for optimized solar absorption.Figure 3b shows the FESEM image of perovskite LSCF nanoparticles revealing the dense morphology of perovskite material with a rough texture to boost the facile light trapping with intrinsic diffuse reflection and promoted enhanced photothermal effect.
Indeed, the open porous assembly appeals to a better capillary action force for excellent water uptake up to the interfacial surface for vapor generation.The FESEM images of the surface structure of LSCF/Ti 3 C 2 reveal plenty of hierarchical micrometer-sized interconnected microchannels to withstand a high potential for quick water supply via capillary force and for vapor generation, as shown in Figure 3c,d.The aligned and ordered symmetry of open pores at both ends of hydrogel ensures efficient water supply, quick vapor escape, and excellent salt rejection.Figure 3e demonstrates the 2D MXene nanosheets embedded in the polymeric network of PVA hydrogel, while the polymeric walls of hydrogels are composed of LSCF/Ti 3 C 2 nanocomposites which can be seen in Figure 3f.Furthermore, the detailed energy dispersive X-ray spectroscopy (EDS) also confirmed the presence of LSCF/Ti 3 C 2 nanocomposites in the polymeric network of PVA hydrogel, as illustrated in Figures S1 and S2 (Supporting Information).The nanocomposite hydrogel depicts the elemental composition which constitutes La, Sr, Co, Fe, Ti, O, N, and C. Additionally, the distribution of LSCF/Ti 3 C 2 into a polymeric network of PVA entails plasmonic localized heating to augment the solar flux capturing for thermal generation.The hierarchical skeleton of a highly porous assembly can efficiently dissolve the salt ions within the matrix to prevent any accumulation inside aligned microchannels.This anisotropic microchannel also bestows good mechanical strength on the aerogel for structural stability.
The efficiency of any designed solar energy-based system greatly relies on its solar light harvesting potential and its photothermal/photochemical conversion with minimum thermal conduction.We developed an efficient LSCF/Ti 3 C 2 -based hydrogel that manifests excellent solar absorption over the entire solar spectral length with good solar-to-thermal and solar-to-chemical energy conversions.The UV-vis spectrum (200-2000 nm) of LSCF and LSCF/Ti 3 C 2 nanocomposite was carried out using UVvis spectroscopy (Figure 4a) which shows LSCF/Ti 3 C 2 nanocomposite exhibits efficient absorption (96%).This efficient absorption potential can be attributed to the localized surface plasmonic The hierarchical porous structure of the LSCF/Ti 3 C 2 hydrogel facilitates the diffuse reflections of incident light inside the dark and porous surface to enhance the solar light harvesting potential.Good thermal control can maximize the efficiency of the overall steam generation system.The thermal conductivity of the fabricated LSCF/Ti 3 C 2 hydrogel was measured experimentally using a thermal conductivity meter (Hot Disk, TPS 2500, Sweden hot disk cooperation).Upon turning on the system, a gradual temperature change (dT/dx) will develop in a vertical direction creating a temperature gradient.This heat transportation rate (q) of the LSCF/Ti 3 C 2 hydrogel can be use understood using Fourier equations [54] Where k 1 shows the thermal conductivity (1.05 W m −1 K −1 ), x 1 shows the width of the glass slide (3 mm), and x 2 is the LSCF/Ti 3 C 2 height (30 mm).Where T 1 is the top surface temperature of the thermal conductivity meter, T 2 and T 3 are the bottoms and top temperatures of the glass slides sandwiching the LSCF/Ti 3 C 2 hydrogel.Finally, the thermal conductivity (k) for LSCF/Ti 3 C 2 hydrogel was computed at the equilibrium point of temperature sustainment and rate by using the following equation The designed LSCF/ Ti 3 C 2 hydrogel shows minimum thermal conductivity in dry conditions (0.15 069 ± 0.00 792 Wm −1 K −1 ) owing to the multiple scattering of incident light to the interior of interfacial surface and transferring their energy in the form of heat to the photothermal surface thereby decreasing the thermal conductivity to the lower matrix of the overall system.The conductivity of the wet LSCF/ Ti 3 C 2 hydrogel was also measured which come out to be much lower than the thermal conduction of water (0.19 626 ± 0.01 315 W m −1 K −1 ) as shown in Figure S3 (Supporting Information).
The interfacial surface temperature enhancement along with minimum thermal conduction plays a decisive role in excellent thermal management.For this, we measured the surface temperatures of the five developed systems, i.e., bulk water, pure PVA, Ti 3 C 2 /PVA, LSCF/PVA, and LSCF/Ti 3 C 2 to compare the heat accumulation potential by recording the surface temperatures under 1 k Wm −2 for 1 h employing two thermocouples positioned on the intended regions, as illustrated in Figure 4c.The LSCF/Ti 3 C 2 hydrogel manifests the maximum solar harvest, excellent flux distribution within the top matrix, and outstanding thermal management which only allows the water conduction up to the top surface and strictly prohibits the downward thermal conduction.Thus, the interfacial photothermal surface increases rapidly up to ≈40.08 °C and finally reached an equilibrium temperature for the top surface of Ti 3 C 2 /LSCF hydrogel showing a good photothermal conversion rate as the underlying water surrounds the Ti 3 C 2 /LSCF below the interfacial layer, which is uptaken via porous assembly and then evaporates via liquid-gas phase change.This high surface temperature attainment enables fast steam generation ultimately leading to high efficiency.The surface temperature of LSCF/Ti 3 C 2 hydrogel was also measured under different simulated solar irradiations and a maximum value of up to 46.27 °C under 3 k Wm −2 irradiations (Figure 4d).
Furthermore, the surface temperature enhancement was also monitored using an infrared (IR) camera for top and cross views under 1 k Wm −2 solar intensity.The LSCF/Ti 3 C 2 (1 cm height and 0.3 cm radius) hydrogel was placed inside a petri dish filled with water under one solar irradiation to capture the temperature for both top and cross surfaces as shown in Figure 5.When the simulated solar intensity was turned on, LSCF/Ti 3 C 2 hydrogel manifests an immediate photothermal conversion on the top surface by absorbing and converting the incident light into heat energy which ultimately leads to an enhancement in the temperature of the top surface.As shown in Figure 5a-f, the top surface of LSCF/Ti 3 C 2 hydrogel shows a temperature change of up to 29.7 °C in the first 15 min which is higher than the ambient temperature.In the next 10 min, the upper surface of achieve an equilibrium temperature of 39.9 °C.Whereas, the temperature of the lower matrix of the LSCF/Ti 3 C 2 hydrogel process maintained a lower temperature value of up to 22 °C throughout this experiment as shown in Figure 5g-l, which was much less than the top surface showing no heat conduction to the downward direction and good thermal insulation for maximum thermal localization on the top surface.The anisotropic low thermal conduction and efficient photothermal conversion of the LSCF/Ti 3 C 2 hydrogel synergically achieve the optimum "Ther-mal localization" to achieve a high evaporation rate.Indeed, good solar absorption and photothermal conversion combined with hydrophilicity are contemplated as primary factors to develop a highly efficient steam generation device.The water contact angle test was performed between the water droplet and the surface of the LSCF/Ti 3 C 2 hydrogel as shown in Figure S4 (Supporting Information), revealing that the LSCF/Ti 3 C 2 hydrogel can be wetted within ≈0.1 s, demonstrating good hydrophilicity for water transport to achieve high evaporation rate.Moreover, mechanical robustness along with good hydrophilicity is an important factor for the selection of any solar steam generation device for longterm sustainability.Figure S5   top surface quickly and constantly which allows fast vapor escape and efficient thermal distribution on the top surface.At the same time, the inner framework of hydrogel lets in enough light for optimal energy absorption and thermal conversion.
The LSCF/Ti 3 C 2 hydrogel was also operated under various solar intensities to check its evaporation potential under higher solar irradiations as shown in Figure 6b.Under 3 k Wm −2 solar intensity, the LSCF/Ti 3 C 2 hydrogel shows an evaporation rate of up to 5.41 kg m −2 h −1 revealing enhanced photothermal response under higher incident light.
The corresponding photothermal conversion efficiency ( evap ) of the LSCF/Ti 3 C 2 hydrogel was measured by the following equation [50,[55][56][57][58] where ṁv is the net evaporation rate (1.98 kg m −2 h −1 ) after substation of evaporation rate under no light condition of bulk water, h LV is the liquid-to-vapor phase change enthalpy, and A evap denotes the evaporation area.Where  here shows latent heat of phase change during the evaporation process (amount of energy required to change the liquid-vapor phase of water during photothermal evaporation) and its value changes at different temperatures (2430 kJ kg −1 K −1 at 30 °C, and 2256 kJ kg −1 K −1 at 100 °C), C is water-specific heat capacity (4.2 kJ kg −1 K −1 ), △T is a temperature difference of water from the initial temperature to the point of vaporization under 1 k Wm −2 (surface temperature increment in the course of photothermal evaporation), and q solar is simulated solar irradiation, which here is estimated up to 1 k Wm −2 .The ambient temperature was 23 ± 1 °C and humidity was 55% while performing experiments.Following these equations (iiiiv), LSCF/Ti 3 C 2 was calculated for an evaporation efficiency up to corresponding photothermal conversion efficiency (90%) excluding optical and heat losses, which is greater than pure water (20%), pure PVA (35%), Ti 3 C 2 /PVA (86%), and LSCF/PVA (88%) as shown in Figure 6c.However, the main hindrance being confronted by evaporation structures is the salt accumulation or structural distortion when operated consistently over a long period which significantly influences the evaporation rate and efficiency of devices.For this, LSCF/Ti 3 C 2 was operated consistently for 8 h under one sun to inspect the smooth evaporation without any structural distortion as shown in Figure 6d.The LSCF/Ti 3 C 2 hydrogel endows smooth mass change (13.33 kg m −2 ) for 8 h of illumination under one sun.Additionally, to quantitatively assess the evaporation performance, cyclic stability, and durability of LSCF/Ti 3 C 2 hydrogel, the evaporation rate was also examined under 1 k Wm −2 over 10 days, as shown in Figure S6 (Supporting Information).A smooth evaporation rate is maintained by LSCF/Ti 3 C 2 hydrogel with no significant shift in slope throughout the operating period confirming the excellent stability of the developed system.The corresponding digital images of the LSCF/Ti 3 C 2 hydrogel are shown in Figure S7 (Supporting Information), reveling no surface degradation after immersing in water for 10 days, exhibiting the good stability of the material and prepared hydrogel in water when operated over a long period.Table 1 represents the comparison of solar evaporation performances with other successful evaporators.Furthermore, the LSCF/Ti 3 C 2 was also operated for salt-rejection potential with no significant impact on evaporation performance under multiple simulated brine solutions, such as 2.5, 5, 10, 15, and 20 wt%, as shown in Figure 6e.
The purifying potential of LSCF/Ti 3 C 2 in the condensed water was examined against the nanofiltration potential for rejection of primary metal ions using inductively coupled plasma-optical emission spectrometry (ICP-OES).Figure 6f demonstrates the primary metal ions, i.e., Na + , K + , Mg 2+ , and Ca 2+ concentration in simulated water and condensed.As obvious, the concentration of ions is reduced significantly in the condensed water and surprisingly much lower than present in the standard drinking water set by World Health Organizations (WHOs).Thus, we have successfully developed an LSCF/Ti 3 C 2 solar evaporator that can be potentially installed for practical applications with no surface degradation and is capable of practical installment at the industrial level for freshwater production.Solar energy, a clean and sustainable power source, is used in the desalination of saltwater.However, because of the high salt content of seawater (3.5 wt% NaCl), the water channels of evaporation structures tend to be blocked during longer operations in colder temperatures.The introduction of novel thin evaporation structures at the expense of thermal insulation is one of several efficient solutions that have recently been suggested to deal with this issue.These thin evaporation structures allow heat to diffuse into the bulk water below from the top interfacial heating layer.The accumulation of salt ultimately prevents the optimization of evaporation efficiency.The self-regeneration and salt rejection potential of the developed solar-driven LSCF/Ti 3 C 2 hydrogel was investigated through different experimental procedures.This was accomplished by placing the LSCF/Ti 3 C 2 hydrogel in a beaker of salt water (3.5 wt% NaCl) and operating it for several hours at 1 sun solar intensity (1 k Wm −2 ), while dispersing 1.  1).

Conclusion
In summary, we successfully designed nanocomposite hydrogel composed of 2D-MXenes nanosheets/perovskite La 0.6 Sr 0.4 Co 0.2 Fe 0.8 O 3− (LSCF) oxide embedded in PVA matrix for efficient solar-driven seawater desalination.The LSCF/Ti 3 C 2 nanocomposite exhibits an aggravated LSPR phenomenon and enhanced surface temperature due to excellent solar absorption (96%).Excellent evaporation rates (1.98 kg m −2 h −1 ) under 1 k Wm −2 solar irradiation are attributed to the microscale thermal confinement through a hierarchical porous network.Several experiments were performed to evaluate the reproducibility, and stability of the evaporation rate without shape distortion, etc.Using LSCF/Ti 3 C 2 hydrogel, we were able to realize the salt-rejection from the top surface (1.2 g NaCl/270 min) without any surface degradation.The present work will provide a techno-economic analysis to determine if the additional cost of implementing outdoor seawater desalination is worthwhile in our future study.The ratio of metal ions and citric acid was fixed as 1:1.5.Afterward, to maintain the pH of the solution, NH 3 was used.Later, the solution was stirred continuously at 80 °C to form a gel and dried at 120 °C for 24 h and followed by sintering the precursor at 1000 °C for 6 h to obtain the LSCF powder.The obtained LSCF powder was ground by putting in a mortar pestle until the formation of fine powder which was saved for characterization and steam generation experimental work.Preparation of Ti 3 C 2 Nanosheets: First of all, 1.0 g of the Ti 3 AlC 2 was mixed into 100 mL of HF and stirred for 72 h at room temperature.Afterward, vacuum filtration was incorporated to separate the resulting suspension.The acquired product was purified using deionized (DI) water to neutralize the pH.Later it was dried in an oven at 60 °C for 12 h to remove volatile impurities.Then, it was removed from the oven and added to 40 mL ethanol followed by 1 h sonication and 10 min centrifuging at 10 000 rpm.The obtained sediments were again dissolved into ethanol (100 mL), sonicated (750 W, 20 min), and centrifuged (3500 rpm, 3 min) to get desired product which was further dried in an oven at 60 °C to obtain the final powder of ultrathin exfoliated Ti 3 C 2 nanosheets.

Experimental Section
LSCF/Ti 3 C 2 Hydrogel: Initially, a stoichiometric amount of PVA (4 g, 10 wt%) was dissolved into the deionized water relatively at a high temperature along with acetic acid to form the homogeneous solution.Then the mixture of LSCF and Ti 3 C 2 with a ratio of 10:1 was added to the PVA mixture with N 2 protection.Afterward, 400 μL hydrochloric acid (HCL, 0.1 wt%) was mixed in the prepared solution followed by adding 195 μL glutaraldehyde (4 wt%) and allowed to gelatinize for 6 h.The obtained hydrogel was washed several times in deionized water to get rid of HCl.Afterward, the obtained hydrogel was frozen and defrosted in water (40 °C) two times until it is ready for testing.
Solar-Driven Evaporation Setup: The solar-driven steam generation performance of the prepared LSCF/Ti 3 C 2 hydrogel was checked by operating it under simulated solar intensity using a solar simulator (PLS-FX300HU) provided with an AM 1.5 solar filter.The intensity of the simulated solar flux was controlled using a CEL-NP2000-2 power meter (Beijing Education Au-light Co., Ltd.).An advanced electronic balance enables measuring with 0.001 g precision (Mettler Toledo, ME204) and was connected to a computer to record the time-dependent mass variations to measure the evaporation rate.The surface temperatures of different systems of the top layer were recorded using two thermocouples (OMEGA, INSP# 33306, 5TC-TT-K-30-197) connected with the acquisition system (KEYSIGHT, 34972A).An inductively coupled plasma-optical emission spectrometry (ICP-OES, EP Optimal 8000) was employed to measure the concentration of primary salt ions in the simulated and condensed water.All the experiments were performed at room temperature of ≈23 °C and humidity level of ≈55-50%.

Figure 5 .
Figure 5. Time-dependent IR images of LSCF/Ti 3 C 2 hydrogel during solar evaporation showing thermal distribution for a-f) top surface and g-i) cross surface.
(Supporting Information) represents the physical robustness test of the LSCF/Ti 3 C 2 which can bear 200 N force without any structural deformation.No surface rupture is observed upon removing the force after 1 h revealing the excellent mechanical stability of our fabricated LSCF/Ti 3 C 2 hydrogel.All these results indicate that LSCF/Ti 3 C 2 hydrogel has good application prospects in photothermal evaporation.The flux distribution on the top surface of LSCF/Ti 3 C 2 hydrogel facilitates the excellent photothermal conversion of incident solar light by inherently dispersing it at the interface, which is the basic mechanism of interfacial solar steam generation.Herein, the developed five evaporation systems (i.e., pure water, pure PVA, Ti 3 C 2 /PVA, LSCF/PVA, and LSCF/Ti 3 C 2 ) were investigated for the continuous vapor generation under 1 k Wm −2 irradiation for 1 h to comparatively analyze their evaporation rate and efficiency.As obvious, the high surface temperature through the LSPR effect with minimum thermal conduction allows enhanced evaporation and elevated evaporation rate.The LSCF/Ti 3 C 2 hydrogel is recorded for an evaporation rate of 1.98 kg m −2 h −1 which is the highest among all the other fabricated systems, i.e., pure water (0.65 kg m −2 h −1 ), pure PVA (0.91 kg m −2 h −1 ), Ti 3 C 2 /PVA (1.64 kg m −2 h −1 ), and LSCF/PVA (1.72 kg m −2 h −1 ) as shown in Figure 6a.In particular, the interconnected water transportation assembly of microspores provides water up to the

Figure 6 .
Figure 6.a) Time-dependent evaporation rate measurement of the developed five systems.b) Evaporation rate evaluation of LSCF/Ti 3 C 2 hydrogel under multiple solar irradiations.c) Comparative evaporation efficiency analysis of the designed systems.d) Long-term mass change of the LSCF/Ti 3 C 2 hydrogel when operated for continuous 8 h under one sun.e) Evaporation rates of LSCF/Ti 3 C 2 hydrogel under different salt concentration solutions.f) Concentrations of primary salt ions in simulated water and condensed water and condensed water when operated using LSCF/Ti 3 C 2 hydrogel.

Figure 7 .
Figure 7. a) Salt-rejection potential of LSCF/Ti 3 C 2 hydrogel to analyze the self-regeneration ability.a−j) 1.2 g of NaCl was spread on the top surface of LSCF/Ti 3 C 2 hydrogel which was completely rejected back to the bulk water through hierarchical porous assembly within 270 min under 1 k Wm −2 solar intensity.
2 g of solid NaCl over the top surface of the LSCF/Ti 3 C 2 hydrogel, as shown in Figure 7a-j.During 4.5 h of continual irradiation, the LSCF/Ti 3 C 2 hydrogel rejected all 1.2 g of solid NaCl, demonstrating excellent great self-regeneration capacity under stable and continuous steam generation.The salt rejection and regeneration capability of the fabricated device is due to the cross-inked and aligned porous structure throughout the hydrogel.Due to the potential gradient created by the different concentrations in the two places, salt ions will be moved from a high-concentration to a low-concentration site by diffusion or convection.The solid NaCl is dissolved by a steady flow of vapor, enabling it to pass through the top surface into the bulk water.The open porous assembly of the LSCF/Ti 3 C 2 hydrogel is orientated to prevent salt accumulation (Table

Table 1 .
Comparison of solar-thermal evaporation performance of LSCF/Ti 3 C 2 hydrogel with other competitive hydrogel-based solar evaporators.